Download presentation

Presentation is loading. Please wait.

Published byGabriella Carr Modified over 2 years ago

1
Announcements 1)Revised Lab timings: 1-3 PM (all groups) 2) Quiz 1, 28 th Jan 2014, Tuesday 7:30 PM, WS 209, WS 213

2
Chapter 3 Crystal Geometry and Structure Determination

3
Recap Lattice, Motif/Basis Crystal = Lattice + Motif e.g. Brass, diamond, ZnS Miller indices of direction: components of vector w.r.t to basis vector a, b and c

4
Miller Indices of directions and planes William Hallowes Miller (1801 – 1880) University of Cambridge

5
5. Enclose in parenthesis Miller Indices for planes 3. Take reciprocal 2. Find intercepts along axes in terms of respective lattice parameters 1. Select a crystallographic coordinate system with origin not on the plane 4. Convert to smallest integers in the same ratio 1 1 1 (111) x y z O

6
Miller Indices for planes (contd.) origin intercepts reciprocals Miller Indices A B C D O ABCD O 1 ∞ ∞ 1 0 0 (1 0 0) OCBE O* 1 -1 ∞ 1 -1 0 (1 1 0) _ Plane x z y O* x z E Zero represents that the plane is parallel to the corresponding axis Bar represents a negative intercept

7
Courtesy: H Bhadhesia

10
Crystallographically equivalent planes

11
Miller indices of a family of symmetry related planes = (hkl ) and all other planes related to (hkl ) by the symmetry of the crystal {hkl } All the faces of the cube are equivalent to each other by symmetry Front & back faces: (100) Left and right faces: (010) Top and bottom faces: (001) {100} = (100), (010), (001)

12
{100} cubic = (100), (010), (001) {100} tetragonal = (100), (010) (001) Cubic Tetragonal Miller indices of a family of symmetry related planes x z y z x y

13
CUBIC CRYSTALS [hkl] (hkl) Angle between two directions [h 1 k 1 l 1 ] and [h 2 k 2 l 2 ]: C [111] (111)

14
Some IMPORTANT Results Weiss zone law True for ALL crystal systems Not in the textbook If a direction [uvw] lies in a plane (hkl) then uh+vk+wl = 0 [uvw] (hkl)

15
d hkl Interplanar spacing between ‘successive’ (hkl) planes passing through the corners of the unit cell O x (100) B O x z E

16
[uvw]Miller indices of a direction (i.e. a set of parallel directions) (hkl)Miller Indices of a plane (i.e. a set of parallel planes) Miller indices of a family of symmetry related directions {hkl}Miller indices of a family of symmetry related planes Summary of Notation convention for Indices

17
How do we determine the structure of a piece of crystalline solid? You can probe the atomic arrangements by X-ray diffraction (XRD)

18
Incident Beam X-Ray Diffraction Transmitted Beam Diffracted Beam Sample Braggs Law (Part 1): For every diffracted beam there exists a set of crystal lattice planes such that the diffracted beam appears to be specularly reflected from this set of planes. ≡ Bragg Reflection

19
Braggs Law (Part 1): the diffracted beam appears to be specularly reflected from a set of crystal lattice planes. Specular reflection: Angle of incidence =Angle of reflection (both measured from the plane and not from the normal) The incident beam, the reflected beam and the plane normal lie in one plane X-Ray Diffraction i plane r

20
X-Ray Diffraction i r d hkl Bragg’s law (Part 2):

21
i r Path Difference =PQ+QR P Q R d hkl

22
Path Difference =PQ+QR i r P Q R Constructive inteference Bragg’s law

23
Extinction Rules: Table 3.3 Bravais LatticeAllowed Reflections SCAll BCC(h + k + l) even FCCh, k and l unmixed DC h, k and l are all odd Or if all are even then (h + k + l) divisible by 4

24
Diffraction analysis of cubic crystals 2 sin 222 )lkh( constant Bragg’s Law: Cubic crystals (1) (2) (2) in (1) =>

25
X Ray Diffractometer

26
You do not get indices of plane!!

27
Cu target, Wavelength = 1.5418 Angstrom 2θ2θ 44.48 51.83 76.35 92.90 98.40 121.87 144.54 Unknown sample, cubic Determine: 1)The crystal structure 2)Lattice parameter

28
5 step program for the determination of crystal structure 1)Start with 2θ values and generate a set of sin 2 θ values 2)Normalise the sin 2 θ values by dividing it with first entry 3)Clear fractions from normalised column: Multiply by common number 4) Speculate on the hkl values that, if expressed as h 2 +k 2 +l 2, would generate the sequence of the “clear fractions” column 5) Compute for each sin 2 θ /(h 2 +k 2 +l 2 ) on the basis of the assumed hkl values. If each entry in this column is identical, then the entire process is validated.

29
2θ2θSin 2 θSin 2 θ/Sin 2 θ 1 Clear fractions (hkl)?sin 2 θ /(h 2 +k 2 +l 2 ) 44.480.1431.0031110.0477 51.830.1911.3442000.0478 76.350.3822.6782200.0478 92.900.5253.67113110.0477 98.400.5734.01122220.0478 121.870.7645.34164000.0477 144.540.9076.34194200.0477

30
William Henry Bragg (1862–1942), William Lawrence Bragg (1890–1971) Nobel Prize (1915) A father-son team that shared a Nobel Prize

31
h 2 + k 2 + l 2 SCFCCBCCDC 1100 2110 3111 4200 5210 6211 7 8220 9300, 221 10310 11311 12222 13320 14321 15 16400 17410, 322 18411, 330 19331

32
Two equivalent ways of stating Bragg’s Law 1 st Form 2 nd Form

33
X-rays Characteristic Radiation, K Target Mo Cu Co Fe Cr Wavelength, Å 0.71 1.54 1.79 1.94 2.29

Similar presentations

OK

Crystallographic Points, Directions, and Planes. ISSUES TO ADDRESS... How to define points, directions, planes, as well as linear, planar, and volume densities.

Crystallographic Points, Directions, and Planes. ISSUES TO ADDRESS... How to define points, directions, planes, as well as linear, planar, and volume densities.

© 2017 SlidePlayer.com Inc.

All rights reserved.

Ads by Google

Ppt on book one minute manager Ppt on social contract theory summary Ppt on trial and error synonyms Ppt on job rotation benefits Ppt on mammals and egg laying animals called Ppt on social etiquettes in india Ppt on led tv technology Ppt on conservation of environment project Ppt on bluetooth technology Ppt on ascending and descending numbers